G2934 Cone 6 Matte Base Glaze G2926B Cone 6 Clear Glossy Base Glaze GA6-B Alberta Slip Cone 6 Base L3954B Mid Temperature Engobe G1916Q Transparent Base Glaze G1947U Transparent Base - Cone 10R G2571A MgO Matte Base - Cone 10R GR10-A Ravenscrag Slip as-a-glaze - Cone 10R L3954N/J Cone 10 Engobe Base
GR10-A Ravenscrag Slip as-a-glaze - Cone 10R
When mixed with water to create a thixotropic slurry, this will perform was as a dipping glaze. It will apply evenly to bisque, produce minimal dripping, dry within seconds and be adequately durable for handling. We document procedures to mix this as a brushing glaze or dipping glaze.
If you are glaze layering (using this as a dipping glaze and painting a commercial gummed brushing glaze over it) there is a risk of crawling. It may be necessary to add some gum to this, converting it from a dipping glaze to a base-coat dipping glaze.
The recipe is 50% raw Ravenscrag Slip and 50% Roast Ravenscrag Slip (see below for info about roasting). More information about this recipe can be found at digitalfire.com, click the following: GR10-A. See also the Ravenscrag Slip page.
This recipe is most often prepared using the traditional method of simply adding water until the desired consistency is achieved (do the initial mix with 8 parts water and 10 powder). No flocculant additions are generally needed and application properties are very good as long as the slurry is not too viscous or too runny (dries quickly without cracking and, after dipping, there is minimal dripping).
Left: Raw Ravenscrag Slip powder. Right: Roasted at 1080F. This is a silty clay, thus it has a relatively low drying shrinkage. Where a glaze is applied thickly or the percentage of Ravenscrag is high, shrinkage cracks (which produce crawling during firing) can occur. We recommend a mix of roast and raw material in recipes. Roasting the Ravenscrag powder at 1000F greatly reduces the shrinkage. Use a firing rate and hold-time-at-1000F appropriate for the wall thickness and size of your bisque vessels (e.g. 500F/hr and 30 minutes for thin walled small vessels, slower and longer hold for large ones). If any of the powder within is black, increase hold time. Adjust proportions as needed (more roast if the glaze cracks on drying or more raw if it is drying too powdery or not bonding well).
P580 with Ravenscrag GR10-A and G1947U (the liner glaze for each). The Ravenscrag is not quite as glossy and it contains enough iron to darken the color of the underlying porcelain. Zircopax could be added to whiten it, however it is best to limit the use of GR10-A to ware that has compatible aesthetics.
Safety Data SheetClick here for web view.
|Plainsman Clays Ltd.|
702 Wood Street, Medicine Hat, Alberta T1A 1E9
Phone: 403-527-8535 FAX:403-527-7508